variation of peak temperature with heating rate in ... of peak temperature with heating rate in...
Post on 06-Mar-2018
Embed Size (px)
Journal 0 f Research of the National Bureau of Standards Vol. 57, No.4, October 1956 Research Paper 2712
Variation of Peak Temperature With Heating Rate In Differential Thermal Analysis
Homer E. Kissinger
In differential thermal analys is, the temp erat ure at which the maxi mum de nection is obse rved varies with h eating rate for certain ty pes of reactio ns. An ex press ion ca n be deri ved r elating this varia t ion with t he kinetics of t lw reaction . By ma king a !lumber of d ir-J'e rential t her mal patterns at dir-J'erent h eating rates, t he kinetic eOJl stants can be obtai ned direeUy from t he differential t hermal data.
Mea surements of t he variation of peak te mperat ure w ith heat illg rate have bee n mad e fo r se veral min erals of t he kaolin group, the valu es of t he kinetic constants dete rmin ed, a lld t hese values compared with corresponding values obtained for both the same samp les and simil ar material by conventional isothermal techniqu es. So me factors affecting t he resul ts are discussed .
The method of difrerential thermal analysis (DT A) has been universally accepted by mineralogi-cal laboratories as a rapid and co nvenient means for recording the thermal effects that occur as a sample is hea ted . Changes in heat content of the active sample arc indi cated by defl ections shown by a line r epresen ting the differen tial temperaturc. It is conven tional to repr-esen t an endothermic eO'ect by a negative deflection and an exothermi c effect by a posi tive deflection . The deflections, whethcr posi tive or negati ve, arc ralleel peaks.
The facLOl's responsible for the si ze, shape, and position of the r csul ting peaks are no t well under-stood. Oft,en (,he ('empera ture of maximum defl ec-Lion , 0 )' peak ('empel'atul'e, is considerably higher than the known transition 0 )' decomposition lem-perature of Lhe subs tance. The penk tempera ture is also markedly an'ected hy changes in techniqu e .1 Only in the case of crystalli ne iLlversions (t,ra nsi-tions occulTing instantaneously at a fi.xed tempera-ture), ha s there been a satisfactory explanation of the DTA peaks .
The work of Murra y and White [3, 4, 5] on the l,inetics of decomposition of clay minera.ls can be appli ed to the interpretation of the DTA patterns of these ma terials. These workers measured the ra tes of isothermal dehydration of clays, calculated the kineti c constants of the materials, and from these data. constructed curves of reaction rate versus time for cons tan thea ting rates. These artificial curves were similar in shape to DTA curv es, the t empera-tures of maximum reaction rate were very close to the pea k temperatures observed in DTA, and these temperatures varied in the same ma nner with heat-ing rate for both the calculated and the observed curves. Later Sewell  found that the pea k tem-peratures of DTA pa tterns mad e at different hea ting rates were predicted fairly closely by the equation of Murray a.nd White.
According to the equation derived by MUlTay and 'White, the temperature of maximum deflection is defin ed by the kinetic constants of the maLerial and
1 Figures iu brackets iud.icate tl1e literature refcrOllees at (he end of this pa per.
the heating rate. The assumption that the peak temperature occurs when the reaction rate is a maximum is supported by the experimental work described above. I t should then be possible to calculate the kinetic constants directly from DT A data by makin g a number of patterns at diA'erent heating rates. The series of experiments to b e described was performed to verify the equation of Murray and Whi te and to apply i t to t ile deter-millation of k ill et ic con tants from DTA data .
2. Preliminary Theory
Murray and White  alld Vaughan  reported that the thermal clecompos i tion of clays obeyed a fU 's t-order law. At constant temperature,
whcre x is the fraction of m.ate rial dccomposed. The magnitude of the ra te co nstant, lc ,l', is determin ed by the tempcratme and is given by the Arrheniu s equation
lc - A - I?'J' 7'- e , (2)
where R is the gas constant, Tis t he Kclvin temper-ature, and A and E are constants that arc properties of the material. The consta.nt E, called the activa-tion energy, is often interpreted as the energy bar-rier opposing the reaction . The constant A , most often called the frequency factor , is a meaSlLl'e of the probability that a molecule having energy E will participate in a reaction.
vv:hen the temperature is changing with time, th e reaction rate is
dX_(OX) +(OX) d1'. dt - ot 7' 01' t dt (3)
The rate of change of x wit h temperature, with the time coordinate fixed, (oX/o1')t is zero, because fixing the time also fixes the number and position of the
particles constituting the sJ:stem. The on~y. effect of an instantaneous change m temperature IS m the vclocity of thermal motion of the particles. The toLal rate of reaction may then be expressed,
dx -R~' dt = A(I - x)e . (4)
This expression holds for any value of T, whether constant or variable, so long as x and T are measured at the same instant.
When the reaction rate is a maximum, its derivative with respect to time is zero. Solving eq (4) for (d /dt ) (dx/elt ):
2 0 0 -
KAOLINIT E A
12 . So/ MIN UTE
DIFFERENTIAL TEMPERATURE 7
600 SAMPL E
TEMPERATURE ~ 4 00
2 0 0
10 20 30 4 0 50 60
it (~~)= ~~ (tr2 ~~ = A e -:T)- (S) FIGURE 1. A typical differentialthermal-analysis pattern of a The maximum value of elx/elt occurs at temperature T m, defined by
_ _ E_ E elT A e RTm _ __ _
- RT;n elt (6)
This is the equation derived by Murray and White .
From eq (6) it is easily seen that
where = elT/elt, the~heating)ate.
3 . Experimental Procedure
3 .1. Materials
The clay minerals of .the kaoli~ groul~ have be.en the predominant mater.lals u.sed.m prevIOUS studws of the relation of chemICal kllletlCs and DT A. For this reason, tbis group has been used in the present study.
Three kaolinite samples, designated A, B, and C, were chosen . Kaolinite A was a Florida kaolinite, whereas Band C were from Georgia. Examination with the electron microscope showed that kaolinites Band C consisted of well formed hexagonal plates with sharply defined edges. The particles of kaoli-nite A were smaller, thicker in proportion to their breadth and less well defined in outline. Impuri-ties wer'e almost nonexistent in all three kaolinites. X-ray examination showed all three to be well crys-tallized with very little b-axis disorder of the type describ~d by Brindley and Robinson .
Two samples of halloysite were chosen, one from Eureka, Utah, and one from Bedford, Ind. These materials were described by Kerr and Kulp . The Indiana material was designated by the symbol H - 12, the Eureka material by H- 13. This identifi-cation was retained for the present study. Both halloysites contained appreciable amounts of impuri-ties, principally gibbsite and quartz.
kaolinite clay. The endothermic peak in th e region 5000 to 7000 0 results from the loss of hy-
droxyl groups from tbe structure. The position, and the helgbt, of tbe peak vary witb heating rate.
3 .2 . Apparatus and Procedure
The differential-thermal-analysis apparatus used in this work consists of a vertical platinum-wound furnace and the associated controlling and recording equipment. Specimen holders are. platinum t';l bes, made of 20-mil Pt sheet. Two SIzes of specImen holders are available, one pair being % in. in diameter by 1 % in . long, the other % in. in diameter .and X in. 10nO'. Platinum-platinum lO-percent-rhodmm ther-mo~ouples made of IS-mil wire are used.
The furnace temperature is con trolled by a cam-driven program controller. A current interrupter in the cam-motor circuit allows any heating rate up to about 2S deg C/min to be selected by the operator.
The differential temperature is measured between the centers of the active and the reference sample . The reference material is a-aluminum oxide. The sample temperature and the differential tempCl~aL1!re are recorded on the same chart by a multlpomt recorder. A typical pattern is s~own in figu~'e ] .
Each of the five sample matenals was run m DT A in the %-in. holders at about 3, 4.S, 6, 10, 12,S , and 20 deg Cimino The 20 deg/min rate was not used with the ~k-in . holders.
Isothermal weight-loss determinations were made wi th the NBS recording analytical balance . A platinum crucible, suspended .in the furnace from one side of the balance, con tams the sample. The loss in weight is recorded continuously while the furnace temperature is held constant. In the present study weight-loss determinations were made at 450, 500 'S500 and 600 C for each material. Approxi-mat~ly 1 g of sample was used for each determina-tion. Reaction-rate constants were calculated at each temperature by the method described by Murray and White . Kinetic constants were then calculated by graphical solution of eq (2).
4 . Results and Discussion The isothermal weight-loss data verified the first-
order law (eq 1) for the three kaolinites. The halloysite decomposition did not obey the first-order
KAOLI NITE B KAOLI NITE C 3 .4
1.08 1.12 1.16 I.oe J.l2 1.16 1.08 1.12 1.16 liT m X 103
FIGURE 2. Differential-thermal-analysis data obtained for the kaolinites in the %-in. specimen holder, plotted to deter-mine E/R.
equation at the higher temperatures . Although other workers [3, 7] have reported that h